- Nano Express
- Open Access
Effect of multilayer structure on high-frequency properties of FeCo/(FeCo)0.63(SiO2)0.37 nanogranular films on flexible substrates
© Zhang et al.; licensee Springer. 2013
- Received: 11 April 2013
- Accepted: 22 April 2013
- Published: 4 May 2013
The high-frequency properties of the FeCo-SiO2 monolayer nanogranular films and FeCo/(FeCo)0.63(SiO2)0.37 multilayer nanogranular films which were elaborated on flexible substrates by magnetron sputtering system were studied. Compared to the monolayer films with the same FeCo content, the multilayer structures comprised of FeCo/(FeCo)0.63(SiO2)0.37 exhibit more excellent properties that the real and imaginary parts of permeability, more than the double value of the monolayer, increase to 250 and 350, respectively. The variation was considered owing to the reduction of the anisotropy field.
- Multilayer film
- High-frequency property
- Flexible substrate
- Anisotropy field
With the rapid increase of demand for the devices used in microwave band, ferromagnetic thin films with the potential for excellent magnetic property in the GHz range, owing to their special structure characteristics and free from Snoek limitation, have been widely studied in recent years.
The basic requirements for magnetic films operated in high frequency are high permeability (μ) and high resistivity (ρ) in GHz range, and metal insulating films, especially Fe and Co based films, have enormous potential to achieve a high permeability, owing to their high saturation magnetization and suitable anisotropic field [1–3]. For the monolayer ferromagnetic films, it is promising to achieve high microwave permeability to increase film thickness. However, the negative influence, the serious skin effect and eddy current [4, 5], and the obvious out-of-plane anisotropy in the high frequency, will block the increasing of the permeability, while the thin magnetic films, with specific multilayer structure design, can efficiently avoid the above negative effect and improve high-frequency properties by leading into different dielectric layers . In this study, FeCo-SiO2 monolayer films and FeCo/(FeCo)0.63(SiO2)0.37 multilayer films were prepared by co-sputtering and tandem sputtering on flexible substrates, respectively, and in order to discuss the improvement of multilayer films, the high-frequency properties of both films whose FeCo content was about 72 at % were investigated.
FeCo-SiO2 monolayer films and FeCo/(FeCo)0.63(SiO2)0.37 multilayer films were all elaborated on flexible substrates by magnetron sputtering system under external bias magnetic field. The flexible substrates of this experiment were 13-μm thick polyethylene terephthalate films. A RF magnetron system was used to sputter SiO2, while DC magnetron cathode was used for FeCo target. The base pressure before deposition was under 1 × 10−7 Torr, and the working pressure during deposition was 2.5 × 10−3 Torr. The difference between the monolayer films and the multilayer films was the sputtering process. The FeCo-SiO2 monolayer films (120 nm) were prepared by co-sputtering both targets all time. For the FeCo/(FeCo)0.63(SiO2)0.37 multilayer films that were prepared by tandem sputtering, FeCo alloy layers (10 nm) and FeCo-SiO2 layers (20 nm) were sputtered alternately by controlling the shutter in front of the Si target. The total thickness of the films was also 120 nm, and the thickness of each layer could be managed by the deposition time.
The structure of the films was investigated by X-ray diffraction (model Bede D1, Durham, England) and transmission electron microscopy (TEM). Saturation magnetization, coercivity, and in-plane magnetic antisotropy field Hk were measured by BHV-525 vibrating sample magnetometer (VSM, Riken Denshi Co., Ltd., Tokyo, Japan). The microstructures and chemical composition of the samples were analyzed using a field emission scanning electron microscope and energy-dispersive spectroscopy. Complex permeability μ was measured in the frequency range of 500 MHz to 8 GHz by coaxial technique. The details of the measurement were discussed before .
It is considered that for the monolayer structure FeCo-SiO2 films, almost the magnetism phase was isolated by non-magnetism phase because the FeCo particles were embedded in SiO2 matrices shown in Figure 1a. The magnetic structure of particles could be regarded as single domains due to the size of the magnetic particles smaller than the critical size of single domain which is dozens of nanometers for Fe65Co3. Thus, the magnetic moment orientation of the single domain was their respective preferred direction and chaotic in plane, and the result relative to high in-plane anisotropy field of the films would improve the resonant frequency and coercivity and reduce the permeability.
Nevertheless, for the multilayer structure FeCo/(FeCo)0.63(SiO2)0.37 films, the domain orientation of individual FeCo layers was consistent owing to the applied magnetic field during sputtering. In order to certify the zero body magnetic charge and minimum magnetostatic energy, two adjacent FeCo layers presented reverse magnetic moment orientation. Meanwhile, the FeCo particles of FeCo-SiO2 layers which were similar to monolayer films could be regarded as single domain particles. However, not as chaotic of the magnetic moment in monolayer films, the magnetic moment orientation of FeCo-SiO2 layers was relatively consistent, which due to the exchange effect and also reported in the Fe65Co35-ZnO films by Wang et al. , which occurred in the several nanometer areas between FeCo and FeCo-SiO2 layers. As a result, the smaller anisotropy field, compared to the monolayer films, would move the resonant frequency to low frequency, reduce the coercivity, and improve the permeability which fits well with the experiment result.
The FeCo-SiO2 monolayer films and FeCo/(FeCo)0.63(SiO2)0.37 multilayer films, with the same FeCo content 72 at %, were all elaborated on flexible substrates by magnetron sputtering system. In both kind of films, the FeCo metal particles are embedded in insulating SiO2matrices and presented polycrystalline structure. Because of the decrease of the anisotropy field by adding FeCo layer, the high-frequency permeability of FeCo/(FeCo)0.63(SiO2)0.37 multilayer films have a huge improvement. Specifically, the real and imaginary parts of permeability, more than the double value of monolayer films, are raised to 250 and 350, respectively. Meanwhile, the coercivity Hc is down to 10 Oe, and the resonant frequency of multilayer films is down to 2.3 GHz.
This work was supported by the National Natural Science Foudation of China (grant no. 51201025) and UESTC Fundamental Research (no. ZYGX2011J032).
- Ge S, Yao D, Yamaguchi M, Yang X: Microstructure and magnetism of FeCo–SiO2 nano-granular films for high frequency application. J Phys D: Appl Phys 2007, 40: 3660–3664. 10.1088/0022-3727/40/12/016View ArticleGoogle Scholar
- Lagarkova AN, Iakubova IT, Ryzhikov IA: Fe-N films: morphology, static and dynamic magnetic properties. Physica B 2007, 394: 159–162. 10.1016/j.physb.2006.12.086View ArticleGoogle Scholar
- Pasquale M, Celegato F, Coisson M: Structure, ferromagnetic resonance, and permeability of nanogranular Fe–Co–B–Ni films. J Appl Phys 2006, 99: 1–3.View ArticleGoogle Scholar
- Acher O, Dubourg S, Duverger F, Malléjac N: GHz permeability of soft CoZr films: the role of exchange–conductivity coupling. J Magn Magn Mater 2007, 310: 2319–2321. 10.1016/j.jmmm.2006.11.029View ArticleGoogle Scholar
- Jeon HJ, Kim I, Kim J, Kim KM, Yamaguchi M: Thickness effect on magnetic properties of nanocrystalline CoFeBN soft magnetic thin films. J Magn Magn Mater 2004, 272–276: 382–384.View ArticleGoogle Scholar
- Chen J, Tang D, Li Y, Zhang B, Yang Y, Lu M, Lu H: High frequency characteristics of NiO/(FeCo/NiO)10 multilayers with exchange anisotropy. J Magn Magn Mater 2010, 322: 3109–3111. 10.1016/j.jmmm.2010.05.039View ArticleGoogle Scholar
- Zhang L, Zhu ZW, Deng LJ: High frequency properties of FeCoB-SiO2 films deposited on flexible substrates. J Appl Supercon Electrom 2009, 1: 155–157.Google Scholar
- Chen CW: Magnetism and Metallurgy of Soft Magnetic Materials. New York: Dover Publications; 1986.Google Scholar
- Wang G, Zhang F, Zuo H, Yu Z, Ge S: Fabrication and magnetic properties of Fe65Co35–ZnO nano-granular films. Nanoscale Res Lett 2010, 5: 1107–1110. 10.1007/s11671-010-9609-yView ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.